Iridium

Iridium is a chemical element; it has symbol Ir and atomic number 77\. This very hard, brittle, silvery-white transition metal of the platinum group, is considered the second-densest naturally occurring metal (after osmium) with a density of 22.56 g/cm3 (0.815 lb/cu in) as defined by experimental X-ray crystallography.[lower-alpha 1] 191Ir and 193Ir are the only two naturally occurring isotopes of iridium, as well as the only stable isotopes; the latter is the more abundant. It is one of the most corrosion-resistant metals, even at temperatures as high as 2,000 °C (3,630 °F).

Iridium was discovered in 1803 in the acid-insoluble residues of platinum ores by the English chemist Smithson Tennant. The name iridium, derived from the Greek word iris (rainbow), refers to the various colors of its compounds. Iridium is one of the rarest elements in Earth's crust, with an estimated annual production of only 6,800 kilograms (15,000 lb) in 2023.

The dominant uses of iridium and its alloys are in high-performance spark plugs, crucibles for recrystallization of semiconductors at high temperatures, and electrodes for the production of chlorine in the chloralkali process. Important compounds of iridium are chlorides and iodides in industrial catalysis. Iridium is a component of some OLEDs.

Iridium is found in meteorites in much higher abundance than in the Earth's crust.[2] For this reason, the unusually high abundance of iridium in the clay layer at the Cretaceous–Paleogene boundary gave rise to the Alvarez hypothesis that the impact of a massive extraterrestrial object caused the extinction of non-avian dinosaurs and many other species 66 million years ago, now known to be produced by the impact that formed the Chicxulub crater. Similarly, an iridium anomaly in core samples from the Pacific Ocean suggested the Eltanin impact of about 2.5 million years ago.[3]

## Contents

* 1 Characteristics
* 1.1 Physical properties
* 1.2 Chemical properties
* 1.3 Isotopes
* 2 Chemistry
* 2.1 Oxidation states
* 2.2 Binary compounds
* 2.3 Complexes
* 2.4 Organoiridium chemistry
* 3 History
* 3.1 Platinum group
* 3.2 Discovery
* 3.3 Metalworking and applications
* 4 Occurrence
* 4.1 Marine oceanography
* 4.2 Cretaceous–Paleogene boundary presence
* 5 Production
* 6 Applications
* 6.1 Metal and alloys
* 6.2 Catalysis
* 6.3 Medical imaging
* 6.4 Photocatalysis and OLEDs
* 6.5 Scientific
* 6.6 Historical
* 7 Precautions and hazards
* 8 Notes
* 9 References
* 10 External links

## Characteristics

### Physical properties

One troy ounce (31.1035 grams) of arc-melted iridium

A member of the platinum group metals, iridium is white, resembling platinum, but with a slight yellowish cast. Because of its hardness, brittleness, and very high melting point, solid iridium is difficult to machine, form, or work; thus powder metallurgy is commonly employed instead.[4] It is the only metal to maintain good mechanical properties in air at temperatures above 1,600 °C (2,910 °F).[5] It has the 10th highest boiling point among all elements and becomes a superconductor at temperatures below 0.14 K (−273.010 °C; −459.418 °F).[6]

Iridium's modulus of elasticity is the second-highest among the metals, being surpassed only by osmium.[5] This, together with a high shear modulus and a very low figure for Poisson's ratio (the relationship of longitudinal to lateral strain), indicate the high degree of stiffness and resistance to deformation that have rendered its fabrication into useful components a matter of great difficulty. Despite these limitations and iridium's high cost, a number of applications have developed where mechanical strength is an essential factor in some of the extremely severe conditions encountered in modern technology.[5]

The measured density of iridium is only slightly lower (by about 0.12%) than that of osmium, the densest metal known.[7][8] Some ambiguity occurred regarding which of the two elements was denser, due to the small size of the difference in density and difficulties in measuring it accurately,[9] but, with increased accuracy in factors used for calculating density, X-ray crystallographic data yielded densities of 22.56 g/cm3 (0.815 lb/cu in) for iridium and 22.59 g/cm3 (0.816 lb/cu in) for osmium.[10]

Iridium is extremely brittle, to the point of being hard to weld because the heat-affected zone cracks, but it can be made more ductile by addition of small quantities of titanium and zirconium (0.2% of each apparently works well).[11]

The Vickers hardness of pure platinum is 56 HV, whereas platinum with 50% of iridium can reach over 500 HV.[12][13]

### Chemical properties

Iridium is the most corrosion-resistant metal known.[14] It is not attacked by acids, including aqua regia, but it can be dissolved in concentrated hydrochloric acid in the presence of sodium perchlorate. In the presence of oxygen, it reacts with cyanide salts.[15] Traditional oxidants also react, including the halogens and oxygen[16] at higher temperatures.[17] Iridium also reacts directly with sulfur at atmospheric pressure to yield iridium disulfide.[18]

### Isotopes

Main article: Physics:Isotopes of iridium

Iridium has two naturally occurring stable isotopes, 191Ir and 193Ir, with natural abundances of 37.3% and 62.7%, respectively.[19] At least 37 radioisotopes have also been synthesized, ranging in mass number from 164 to 202. 192Ir, which falls between the two stable isotopes, is the most stable radioisotope, has a half-life of 73.82 days, and finds application in brachytherapy[20] and in industrial radiography, particularly for nondestructive testing of welds in steel in the oil and gas industries; iridium-192 sources have been involved in a number of radiological accidents. Three other isotopes have half-lives of at least a day—188Ir, 189Ir, and 190Ir.[19] Isotopes with masses below 191 decay by some combination of β+ decay, α decay, and (rare) proton emission. Synthetic isotopes heavier than 193 decay by β− decay, and 192Ir has both, but β+ decay (95.24%) dominates over electron capture (4.76%).[19]

At least 32 metastable isomers have been characterized, ranging in mass number from 164 to 197. The most stable of these is 192m2Ir, which decays by isomeric transition with a half-life of 241 years,[19] making it more stable than any of iridium's ground-state radioisotopes.

The isotope 191Ir was the first one of any element to be shown to present a Mössbauer effect. This renders it useful for Mössbauer spectroscopy for research in physics, chemistry, biochemistry, metallurgy, and mineralogy.[21]

## Chemistry

See also: Chemistry:Iridium compounds

Oxidation states[lower-alpha 2]

−3 | [Ir(CO)3]3−
−1 | [Ir(CO)
3(PPh
3)]1−
0 | Ir
4(CO)

+1 | [IrCl(CO)(PPh

+2 | Ir(C

+3 | IrCl

+4 | IrO

+5 | Ir

+6 | IrF6
+7 | [Ir(O
2)O
2]+

+8 | IrO

+9 | [IrO
4]+
[22]

### Oxidation states

Iridium forms compounds in oxidation states between −3 and +9, but the most common oxidation states are +1, +2, +3, and +4.[4] Well-characterized compounds containing iridium in the +6 oxidation state include IrF
6 and the oxides Sr
2MgIrO
6 and Sr
2CaIrO
6.[4][23] Iridium(VIII) oxide (IrO
4) was generated under matrix isolation conditions at 6 K in argon.[24] The highest oxidation state (+9), which is also the highest recorded for any element, is found in gaseous [IrO
4]+
.[22]

### Binary compounds

Iridium does not form binary hydrides. Only one binary oxide is well-characterized: iridium dioxide, IrO2. It is a blue black solid that adopts the fluorite structure.[4] A sesquioxide, Ir2O3, has been described as a blue-black powder, which is oxidized to IrO2 by HNO3.[16] The corresponding disulfides, diselenides, sesquisulfides, and sesquiselenides are known, as well as IrS3.[4]

Binary trihalides, IrX3, are known for all of the halogens.[4] For oxidation states +4 and above, only the tetrafluoride, pentafluoride and hexafluoride are known.[4] Iridium hexafluoride, IrF6, is a volatile yellow solid, composed of octahedral molecules. It decomposes in water and is reduced to IrF4.[4] Iridium pentafluoride is also a strong oxidant, but it is a tetramer, Ir4F20, formed by four corner-sharing octahedra.[4]

### Complexes

Hydrated iridium trichloride, a common salt of iridium.

Iridium has extensive coordination chemistry.

Iridium in its complexes is always low-spin. Ir(III) and Ir(IV) generally form octahedral complexes.[4] Polyhydride complexes are known for the +5 and +3 oxidation states.[25] One example is IrH
5(PiPr

2 (iPr = isopropyl).[26] The ternary hydride Mg6Ir2H11 is believed to contain both the IrH4−5 and the 18-electron IrH5−4 anion.[27]

Iridium also forms oxyanions with oxidation states +4 and +5. K2IrO3 and KIrO3 can be prepared from the reaction of potassium oxide or potassium superoxide with iridium at high temperatures. Such solids are not soluble in conventional solvents.[28]

Just like many elements, iridium forms important chloride complexes. Hexachloroiridic (IV) acid, H2IrCl6, and its ammonium salt are common iridium compounds from both industrial and preparative perspectives.[29] They are intermediates in the purification of iridium and used as precursors for most other iridium compounds, as well as in the preparation of anode coatings. The IrCl2−6 ion has an intense dark brown color, and can be readily reduced to the lighter-colored IrCl3−6 and vice versa.[29] Iridium trichloride, IrCl3, which can be obtained in anhydrous form from direct oxidation of iridium powder by chlorine at 650 °C,[29] or in hydrated form by dissolving Ir2O3 in hydrochloric acid, is often used as a starting material for the synthesis of other Ir(III) compounds.[4] Another compound used as a starting material is potassium hexachloroiridate(III), K
3IrCl
6.[30]

### Organoiridium chemistry

Cyclooctadiene iridium chloride dimer is a common complex of Ir(I).

Organoiridium compounds contain iridium–carbon bonds. Early studies identified the very stable tetrairidium dodecacarbonyl, Ir4(CO)12.[4] In this compound, each of the iridium atoms is bonded to the other three, forming a tetrahedral cluster. The discovery of Vaska's complex (IrCl(CO)[P(C6H5)3]2) opened the door for oxidative addition reactions, a process fundamental to useful reactions. For example, Crabtree's catalyst, a homogeneous catalyst for hydrogenation reactions.[31][32]

Oxidative addition to hydrocarbons in organoiridium chemistry[33][34]

Iridium complexes played a pivotal role in the development of carbon–hydrogen bond activation (C–H activation), which promises to allow functionalization of hydrocarbons, which are traditionally regarded as unreactive.[35]

## History

### Platinum group

The Greek goddess Iris, after whom iridium was named.

The discovery of iridium is intertwined with that of platinum and the other metals of the platinum group. The first European reference to platinum appears in 1557 in the writings of the Italian humanist Julius Caesar Scaliger as a description of an unknown noble metal found between Darién and Mexico, "which no fire nor any Spanish artifice has yet been able to liquefy".[36] From their first encounters with platinum, the Spanish generally saw the metal as a kind of impurity in gold, and it was treated as such. It was often simply thrown away, and there was an official decree forbidding the adulteration of gold with platinum impurities.[37]

This alchemical symbol for platinum was made by joining the symbols of silver (moon) and gold (sun). Antonio de Ulloa is credited in European history with the discovery of platinum.

In 1735, Antonio de Ulloa and Jorge Juan y Santacilia saw Native Americans mining platinum while the Spaniards were travelling through Colombia and Peru for eight years. Ulloa and Juan found mines with the whitish metal nuggets and took them home to Spain. Ulloa returned to Spain and established the first mineralogy lab in Spain and was the first to systematically study platinum, which was in 1748. His historical account of the expedition included a description of platinum as being neither separable nor calcinable. Ulloa also anticipated the discovery of platinum mines. After publishing the report in 1748, Ulloa did not continue to investigate the new metal. In 1758, he was sent to superintend mercury mining operations in Huancavelica.[36]

In 1741, Charles Wood,[38] a British metallurgist, found various samples of Colombian platinum in Jamaica, which he sent to William Brownrigg for further investigation.

In 1750, after studying the platinum sent to him by Wood, Brownrigg presented a detailed account of the metal to the Royal Society, stating that he had seen no mention of it in any previous accounts of known minerals.[39] Brownrigg also made note of platinum's extremely high melting point and refractory metal-like behaviour toward borax. Other chemists across Europe soon began studying platinum, including Andreas Sigismund Marggraf,[40] Torbern Bergman, Jöns Jakob Berzelius, William Lewis, and Pierre Macquer. In 1752, Henrik Scheffer published a detailed scientific description of the metal, which he referred to as "white gold", including an account of how he succeeded in fusing platinum ore with the aid of arsenic. Scheffer described platinum as being less pliable than gold, but with similar resistance to corrosion.[36]

### Discovery

Chemists who studied platinum dissolved it in aqua regia (a mixture of hydrochloric and nitric acids) to create soluble salts. They always observed a small amount of a dark, insoluble residue.[5] Joseph Louis Proust thought that the residue was graphite.[5] The French chemists Victor Collet-Descotils, Antoine François, comte de Fourcroy, and Louis Nicolas Vauquelin also observed the black residue in 1803, but did not obtain enough for further experiments.[5]

In 1803 British scientist Smithson Tennant (1761–1815) analyzed the insoluble residue and concluded that it must contain a new metal. Vauquelin treated the powder alternately with alkali and acids[14] and obtained a volatile new oxide, which he believed to be of this new metal—which he named ptene, from the Greek word πτηνός ptēnós, "winged".[41][42] Tennant, who had the advantage of a much greater amount of residue, continued his research and identified the two previously undiscovered elements in the black residue, iridium and osmium.[5][14] He obtained dark red crystals (probably of Na2[IrCl6]·nH2O) by a sequence of reactions with sodium hydroxide and hydrochloric acid.[42] He named iridium after Iris (Ἶρις), the Greek winged goddess of the rainbow and the messenger of the Olympian gods, because many of the salts he obtained were strongly colored.[lower-alpha 3][43] Discovery of the new elements was documented in a letter to the Royal Society on June 21, 1804.[5][44]

### Metalworking and applications

British scientist John George Children was the first to melt a sample of iridium in 1813 with the aid of "the greatest galvanic battery that has ever been constructed" (at that time).[5] The first to obtain high-purity iridium was Robert Hare in 1842. He found it had a density of around 21.8 g/cm3 (0.79 lb/cu in) and noted the metal is nearly immalleable and very hard. The first melting in appreciable quantity was done by Henri Sainte-Claire Deville and Jules Henri Debray in 1860. They required burning more than 300 litres (79 US gal) of pure O2 and H2 gas for each 1 kilogram (2.2 lb) of iridium.[5]

These extreme difficulties in melting the metal limited the possibilities for handling iridium. John Isaac Hawkins was looking to obtain a fine and hard point for fountain pen nibs, and in 1834 managed to create an iridium-pointed gold pen. In 1880, John Holland and William Lofland Dudley were able to melt iridium by adding phosphorus and patented the process in the United States; British company Johnson Matthey later stated they had been using a similar process since 1837 and had already presented fused iridium at a number of World Fairs.[5] The first use of an alloy of iridium with ruthenium in thermocouples was made by Otto Feussner in 1933. These allowed for the measurement of high temperatures in air up to 2,000 °C (3,630 °F).[5]

In Munich, Germany in 1957 Rudolf Mössbauer, in what has been called one of the "landmark experiments in twentieth-century physics",[45] discovered the resonant and recoil-free emission and absorption of gamma rays by atoms in a solid metal sample containing only 191Ir.[46] This phenomenon, known as the Mössbauer effect resulted in the awarding of the Nobel Prize in Physics in 1961, at the age 32, just three years after he published his discovery.[47]

## Occurrence

Along with many elements having atomic weights higher than that of iron, iridium is only naturally formed by the r-process (rapid neutron capture) in neutron star mergers and possibly rare types of supernovae.[48][49][50]

Iridium is one of the least abundant elements in Earth's crust. The Willamette Meteorite, the sixth-largest meteorite found in the world, has 4.7 ppm iridium.[51]

Iridium is one of the nine least abundant stable elements in Earth's crust, having an average mass fraction of 0.001 ppm in crustal rock; gold is 4 times more abundant, platinum is 10 times more abundant, silver and mercury are 80 times more abundant.[4] Osmium, tellurium, ruthenium, rhodium and rhenium are about as abundant as iridium.[52] In contrast to its low abundance in crustal rock, iridium is relatively common in meteorites, with concentrations of 0.5 ppm or more.[53] The overall concentration of iridium on Earth is thought to be much higher than what is observed in crustal rocks, but because of the density and siderophilic ("iron-loving") character of iridium, it descended below the crust and into Earth's core when the planet was still molten.[29]

Iridium is found in nature as an uncombined element or in natural alloys, especially the iridium–osmium alloys osmiridium (osmium-rich) and iridosmium (iridium-rich).[14] In nickel and copper deposits, the platinum group metals occur as sulfides, tellurides, antimonides, and arsenides. In all of these compounds, platinum can be exchanged with a small amount of iridium or osmium. As with all of the platinum group metals, iridium can be found naturally in alloys with raw nickel or raw copper.[54] A number of iridium-dominant minerals, with iridium as the species-forming element, are known. They are exceedingly rare and often represent the iridium analogues of the above-given ones. The examples are irarsite and cuproiridsite, to mention some.[55][56][57] Within Earth's crust, iridium is found at highest concentrations in three types of geologic structure: igneous deposits (crustal intrusions from below), impact craters, and deposits reworked from one of the former structures. The largest known primary reserves are in the Bushveld igneous complex in South Africa,[58] (near the largest known impact structure, the Vredefort impact structure) though the large copper–nickel deposits near Norilsk in Russia, and the Sudbury Basin (also an impact crater) in Canada are also significant sources of iridium. Smaller reserves are found in the United States.[58] Iridium is also found in secondary deposits, combined with platinum and other platinum group metals in alluvial deposits. The alluvial deposits used by pre-Columbian people in the Chocó Department of Colombia are still a source for platinum-group metals. As of 2003, world reserves have not been estimated.[14]

### Marine oceanography

Iridium is found within marine organisms, sediments, and the water column. The abundance of iridium in seawater[59] and organisms[60] is relatively low, as it does not readily form chloride complexes.[60] The abundance in organisms is about 20 parts per trillion, or about five orders of magnitude less than in sedimentary rocks at the Cretaceous–Paleogene (K–T) boundary.[60] The concentration of iridium in seawater and marine sediment is sensitive to marine oxygenation, seawater temperature, and various geological and biological processes.[61]

Iridium in sediments can come from cosmic dust, volcanoes, precipitation from seawater, microbial processes, or hydrothermal vents,[61] and its abundance can be strongly indicative of the source.[62][61] It tends to associate with other ferrous metals in manganese nodules.[59] Iridium is one of the characteristic elements of extraterrestrial rocks, and, along with osmium, can be used as a tracer element for meteoritic material in sediment.[63][64] For example, core samples from the Pacific Ocean with elevated iridium levels suggested the Eltanin impact of about 2.5 million years ago.[3]

Some of the mass extinctions, such as the Cretaceous extinction, can be identified by anomalously high concentrations of iridium in sediment, and these can be linked to major asteroid impacts.[65]

### Cretaceous–Paleogene boundary presence

The red arrow points to the Cretaceous–Paleogene boundary.

Main article: Earth:Cretaceous–Paleogene extinction event

The Cretaceous–Paleogene boundary of 66 million years ago, marking the temporal border between the Cretaceous and Paleogene periods of geological time, was identified by a thin stratum of iridium-rich clay.[66] A team led by Luis Alvarez proposed in 1980 an extraterrestrial origin for this iridium, attributing it to an asteroid or comet impact.[66] Their theory, known as the Alvarez hypothesis, is now widely accepted to explain the extinction of the non-avian dinosaurs. A large buried impact crater structure with an estimated age of about 66 million years was later identified under what is now the Yucatán Peninsula (the Chicxulub crater).[67][68] Dewey M. McLean and others argue that the iridium may have been of volcanic origin instead, because Earth's core is rich in iridium, and active volcanoes such as Piton de la Fournaise, in the island of Réunion, are still releasing iridium.[69][70]

## Production

Year | Consumption
(tonnes) | Price (US$)[71]

|
|

2001 | 2.6 | $415.25/ozt ($13.351/g)
2002 | 2.5 | $294.62/ozt ($9.472/g)
2003 | 3.3 | $93.02/ozt ($2.991/g)
2004 | 3.60 | $185.33/ozt ($5.958/g)
2005 | 3.86 | $169.51/ozt ($5.450/g)
2006 | 4.08 | $349.45/ozt ($11.235/g)
2007 | 3.70 | $444.43/ozt ($14.289/g)
2008 | 3.10 | $448.34/ozt ($14.414/g)
2009 | 2.52 | $420.4/ozt ($13.52/g)
2010 | 10.40 | $642.15/ozt ($20.646/g)
2011 | 9.36 | $1,035.87/ozt ($33.304/g)
2012 | 5.54 | $1,066.23/ozt ($34.280/g)
2013 | 6.16 | $826.45/ozt ($26.571/g)
2014 | 6.1 | $556.19/ozt ($17.882/g)
2015 | 7.81 | $544/ozt ($17.5/g)
2016 | 7.71 | $586.90/ozt ($18.869/g)
2017 | n.d. | $908.35/ozt ($29.204/g)
2018 | n.d. | $1,293.27/ozt ($41.580/g)
2019 | n.d. | $1,485.80/ozt ($47.770/g)
2020 | n.d. | $1,633.51/ozt ($52.519/g)
2021 | n.d. | $5,400.00/ozt ($173.614/g)
2022 | n.d. | $3,980.00/ozt ($127.960/g)
2023 | n.d. | $4,652.38/ozt ($149.577/g)
2024 | n.d. | $5,000.00/ozt ($160.754/g)

Worldwide production of iridium was about 7,300 kilograms (16,100 lb) in 2018.[72] The price is high and varying (see table). Illustrative factors that affect the price include oversupply of Ir crucibles[71][73] and changes in LED technology.[74]

Platinum metals occur together as dilute ores. Iridium is one of the rarer platinum metals: for every 190 tonnes of platinum obtained from ores, only 7.5 tonnes of iridium is isolated.[75] To separate the metals, they must first be brought into solution. Two methods for rendering Ir-containing ores soluble are (i) fusion of the solid with sodium peroxide followed by extraction of the resulting glass in aqua regia and (ii) extraction of the solid with a mixture of chlorine with hydrochloric acid.[29][58] From soluble extracts, iridium is separated by precipitating solid ammonium hexachloroiridate ((NH4)2IrCl6) or by extracting IrCl2−6 with organic amines.[76] The first method is similar to the procedure Tennant and Wollaston used for their original separation. The second method can be planned as continuous liquid–liquid extraction and is therefore more suitable for industrial scale production. In either case, the product, an iridium chloride salt, is reduced with hydrogen, yielding the metal as a powder or sponge, which is amenable to powder metallurgy techniques.[77][78] Iridium is also obtained commercially as a by-product from nickel and copper mining and processing. During electrorefining of copper and nickel, noble metals such as silver, gold and the platinum group metals as well as selenium and tellurium settle to the bottom of the cell as anode mud, which forms the starting point for their extraction.[71]

Leading iridium-producing countries (kg)[79] Country | 2016 | 2017 | 2018 | 2019 | 2020

|
|
|
|
|

World | 7,720 | 7,180 | 7,540 | 7,910 | 8,170
South Africa | 6,624 | 6,057 | 6,357 | 6,464 | 6,786
Zimbabwe | 598 | 619 | 586 | 845 | 836
Canada | 300 | 200 | 400 | 300 | 300
Russia | 200 | 300 | 200 | 300 | 250

## Applications

Due to iridium's resistance to corrosion it has industrial applications. The main areas of use are electrodes for producing chlorine and other corrosive products, OLEDs, crucibles, catalysts (e.g. acetic acid), and ignition tips for spark plugs.[75]

### Metal and alloys

Resistance to heat and corrosion are the bases for several uses of iridium and its alloys.

Owing to its high melting point, hardness, and corrosion resistance, iridium is used to make crucibles. Such crucibles are used in the Czochralski process to produce oxide single-crystals (such as sapphires) for use in computer memory devices and in solid state lasers.[80][81] The crystals, such as gadolinium gallium garnet and yttrium gallium garnet, are grown by melting pre-sintered charges of mixed oxides under oxidizing conditions at temperatures up to 2,100 °C (3,810 °F).[5]

Certain long-life aircraft engine parts are made of an iridium alloy, and an iridium–titanium alloy is used for deep-water pipes because of its corrosion resistance.[14] Iridium is used for multi-pored spinnerets, through which a plastic polymer melt is extruded to form fibers, such as rayon.[82] Osmium–iridium is used for compass bearings and for balances.[5]

Because of their resistance to arc erosion, iridium alloys are used by some manufacturers for the centre electrodes of spark plugs,[80][83] and iridium-based spark plugs are particularly used in aviation.

### Catalysis

Iridium compounds are used as catalysts in the Cativa process for carbonylation of methanol to produce acetic acid.[84][85]

Iridium complexes are often active for asymmetric hydrogenation both by traditional hydrogenation.[86] and transfer hydrogenation.[87] This property is the basis of the industrial route to the chiral herbicide (S)-metolachlor. As practiced by Syngenta on the scale of 10,000 tons/year, the complex [Ir(COD)Cl]2 in the presence of Josiphos ligands.[88]

### Medical imaging

The radioisotope iridium-192 is one of the two most important sources of energy for use in industrial γ-radiography for non-destructive testing of metals.[89][90] Additionally, The element Chemistry:Ir does not exist. is used as a source of gamma radiation for the treatment of cancer using brachytherapy, a form of radiotherapy where a sealed radioactive source is placed inside or next to the area requiring treatment. Specific treatments include high-dose-rate prostate brachytherapy, biliary duct brachytherapy, and intracavitary cervix brachytherapy.[14] Iridium-192 is normally produced by neutron activation of isotope iridium-191 in natural-abundance iridium metal.[91]

### Photocatalysis and OLEDs

Iridium complexes are key components of white OLEDs. Similar complexes are used in photocatalysis.[92]

### Scientific

International Prototype Meter bar

An alloy of 90% platinum and 10% iridium was used in 1889 to construct the International Prototype Meter and kilogram mass, kept by the International Bureau of Weights and Measures near Paris.[14] The meter bar was replaced as the definition of the fundamental unit of length in 1960 by a line in the atomic spectrum of krypton,[lower-alpha 4][93] but the kilogram prototype remained the international standard of mass until 20 May 2019, when the kilogram was redefined in terms of the Planck constant.[94]

### Historical

Fountain pen nib labelled Iridium Point

Iridium–osmium alloys were previously used in fountain pen nib tips. The first major use of iridium was in 1834 in nibs mounted on gold.[5] Starting in 1944, the Parker 51 fountain pen was fitted with a nib tipped by a ruthenium and iridium alloy (with 3.8% iridium). The tip material in modern fountain pens is still conventionally called "iridium", although there is seldom any iridium in it; other metals such as ruthenium, osmium, and tungsten have taken its place.[95]

An iridium–platinum alloy was used for the touch holes or vent pieces of cannon. According to a report of the Paris Exhibition of 1867, one of the pieces being exhibited by Johnson and Matthey "has been used in a Whitworth gun for more than 3000 rounds, and scarcely shows signs of wear yet. Those who know the constant trouble and expense which are occasioned by the wearing of the vent-pieces of cannon when in active service, will appreciate this important adaptation".[96]

The pigment iridium black, which consists of very finely divided iridium, is used for painting porcelain an intense black; it was said that "all other porcelain black colors appear grey by the side of it".[97]

## Precautions and hazards

Iridium in bulk metallic form is not biologically important or hazardous to health due to its lack of reactivity with tissues; there are only about 20 parts per trillion of iridium in human tissue.[14] Like most metals, finely divided iridium powder can be hazardous to handle, as it is an irritant and may ignite in air.[58] Iridium is relatively unhazardous otherwise, with the only effect of Iridium ingestion being irritation of the digestive tract.[98] However, soluble salts, such as the iridium halides, could be hazardous due to elements other than iridium or due to iridium itself.[20] At the same time, most iridium compounds are insoluble, which makes absorption into the body difficult.[14]

A radioisotope of iridium, 192Ir, is dangerous, like other radioactive isotopes. The only reported injuries related to iridium concern accidental exposure to radiation from 192Ir used in brachytherapy.[20] High-energy gamma radiation from 192Ir can increase the risk of cancer. External exposure can cause burns, radiation poisoning, and death. Ingestion of 192Ir can burn the linings of the stomach and the intestines.[99] 192Ir, 192mIr, and 194mIr tend to deposit in the liver, and can pose health hazards from both gamma and beta radiation.[53]

## Notes

1. ↑ At room temperature and standard atmospheric pressure, iridium has been calculated to have a density of 22.65 g/cm3 (0.818 lb/cu in), 0.04 g/cm3 (0.0014 lb/cu in) higher than osmium measured the same way. Still, the experimental X-ray crystallography value is considered to be the most accurate, and as such iridium is considered to be the second densest element.[1]
2. ↑ Most common oxidation states of iridium are in bold. The right column lists one representative compound for each oxidation state.
3. ↑ Iridium literally means "of rainbows".
4. ↑ The definition of the meter was changed again in 1983. The meter is currently defined as the distance traveled by light in a vacuum during a time interval of ​1⁄299,792,458 of a second.

## References

1. ↑ Arblaster, J. W. (1989). "Densities of Osmium and Iridium Recalculations Based upon a Review of the Latest Crystallographic Data". Platinum Metals Rev. 33 (1): 14–16. doi:10.1595/003214089X3311416. https://www.technology.matthey.com/article/33/1/14-16/.
2. ↑ Becker, Luann (2002). "Repeated Blows". Scientific American 286 (3): 77–83. doi:10.1038/scientificamerican0302-76. PMID 11857903. Bibcode: 2002SciAm.286c..76B. http://www.miracosta.edu/home/kmeldahl/articles/blows.pdf. Retrieved January 19, 2016.
3. ↑ 3.0 3.1 Kyte, Frank T.; Zhiming Zhou; John T. Wasson (1981). "High noble metal concentrations in a late Pliocene sediment". Nature 292 (5822): 417–420. doi:10.1038/292417a0. ISSN 0028-0836. Bibcode: 1981Natur.292..417K.
4. ↑ 4.00 4.01 4.02 4.03 4.04 4.05 4.06 4.07 4.08 4.09 4.10 4.11 4.12 Greenwood, N. N.; Earnshaw, A. (1997). Chemistry of the Elements (2nd ed.). Oxford: Butterworth–Heinemann. pp. 1113–1143, 1294. ISBN 978-0-7506-3365-9. OCLC 213025882.
5. ↑ 5.00 5.01 5.02 5.03 5.04 5.05 5.06 5.07 5.08 5.09 5.10 5.11 5.12 5.13 5.14 Hunt, L. B. (1987). "A History of Iridium". Platinum Metals Review 31 (1): 32–41. doi:10.1595/003214087X3113241. https://technology.matthey.com/documents/496120/626258/pmr-v31-i1-032-041.pdf/. Retrieved 2022-09-29.
6. ↑ Kittel, C. (2004). Introduction to Solid State Physics (7th ed.). Wiley-India. ISBN 978-81-265-1045-0.
7. ↑ Arblaster, J. W. (1995). "Osmium, the Densest Metal Known". Platinum Metals Review 39 (4): 164. doi:10.1595/003214095X394164164. http://www.platinummetalsreview.com/dynamic/article/view/pmr-v39-i4-164-164. Retrieved 2008-10-02.
8. ↑ Cotton, Simon (1997). Chemistry of Precious Metals. Springer-Verlag New York, LLC. p. 78. ISBN 978-0-7514-0413-5.
9. ↑ Lide, D. R. (1990). CRC Handbook of Chemistry and Physics. (70th ed.). Boca Raton (FL):CRC Press. ISBN 9780849304712. https://archive.org/details/crchandbookofche00lide.
10. ↑ Arblaster, J. W. (1989). "Densities of osmium and iridium: recalculations based upon a review of the latest crystallographic data". Platinum Metals Review 33 (1): 14–16. doi:10.1595/003214089X3311416. https://technology.matthey.com/article/33/1/14-16/. Retrieved 2008-09-17.
11. ↑ & Rhys, David US patent 3293031A, published 20/12/1966
12. ↑ Darling, A. S. (1960). "Iridium Platinum Alloys – A Critical Review Of Their Constitution And Properties". Platinum Metals Review 4 (1): 18–26. doi:10.1595/003214060X411826. https://technology.matthey.com/article/4/1/18-26/. Reviewed in "Iridium–Platinum Alloys". Nature 186 (4720): 211. 1960. doi:10.1038/186211a0. Bibcode: 1960Natur.186Q.211..
13. ↑ Biggs, T.; Taylor, S. S.; van der Lingen, E. (2005). "The Hardening of Platinum Alloys for Potential Jewellery Application". Platinum Metals Review 49 (1): 2–15. doi:10.1595/147106705X24409.
14. ↑ 14.00 14.01 14.02 14.03 14.04 14.05 14.06 14.07 14.08 14.09 Emsley, J. (2003). "Iridium". Nature's Building Blocks: An A–Z Guide to the Elements. Oxford, England, UK: Oxford University Press. pp. 201–204. ISBN 978-0-19-850340-8. https://archive.org/details/naturesbuildingb0000emsl/page/201.
15. ↑ Emsley, John (2011). Nature's Building Blocks: An A–Z Guide to the Elements (New ed.). New York: Oxford University Press. ISBN 978-0-19-960563-7.
16. ↑ 16.0 16.1 Perry, D. L. (1995). Handbook of Inorganic Compounds. CRC Press. pp. 203–204. ISBN 978-1439814611.
17. ↑ Lagowski, J. J., ed (2004). Chemistry Foundations and Applications. 2. Thomson Gale. pp. 250–251. ISBN 978-0028657233. https://archive.org/details/chemistryfoundat0000unse/page/250.
18. ↑ "The Synthesis of Iridium Disulfide and Nickel diarsenide having the Pyrite Structure". Inorganic Chemistry 7 (2): 389–390. February 1968. doi:10.1021/ic50060a047. https://htracyhall.org/ocr/HTH-Archives/Cabinet 8/Drawer 3 (MATI - MOZ)/(Munson, R.A.) (Muntoni, C.) (Murase, K.) (linked)/(Munson, R.A.) (Muntoni, C.) (Murase, K.)-237_OCR.pdf. Retrieved 2019-01-19.
19. ↑ 19.0 19.1 19.2 19.3 Kondev, F. G.; Wang, M.; Huang, W. J.; Naimi, S.; Audi, G. (2021). "The NUBASE2020 evaluation of nuclear properties". Chinese Physics C 45 (3). doi:10.1088/1674-1137/abddae. https://www-nds.iaea.org/amdc/ame2020/NUBASE2020.pdf.
20. ↑ 20.0 20.1 20.2 Mager Stellman, J. (1998). "Iridium". Encyclopaedia of Occupational Health and Safety. International Labour Organization. pp. 63.19. ISBN 978-92-2-109816-4. OCLC 35279504. https://books.google.com/books?id=nDhpLa1rl44C&pg=PT125.
21. ↑ Chereminisoff, N. P. (1990). Handbook of Ceramics and Composites. CRC Press. p. 424. ISBN 978-0-8247-8006-7.
22. ↑ 22.0 22.1 Cite error: Invalid `<ref>` tag; no text was provided for refs named `IrIX`
23. ↑ Jung, D.; Demazeau, Gérard (1995). "High Oxygen Pressure and the Preparation of New Iridium (VI) Oxides with Perovskite Structure: Sr2MIrO6 (M = Ca, Mg)". Journal of Solid State Chemistry 115 (2): 447–455. doi:10.1006/jssc.1995.1158. Bibcode: 1995JSSCh.115..447J.Sr2MIrO6+(M+=+Ca,+Mg)&rft.jtitle=Journal+of+Solid+State+Chemistry&rft.aulast=Jung&rft.aufirst=D.&rft.au=Jung, D.&rft.au=Demazeau, Gérard&rft.date=1995&rft.volume=115&rft.issue=2&rft.pages=447–455&rft_id=info:doi/10.1006/jssc.1995.1158&rft_id=info:bibcode/1995JSSCh.115..447J&rfr_id=info:sid/en.wikibooks.org:Chemistry:Iridium">
24. ↑ Gong, Y.; Zhou, M.; Kaupp, M.; Riedel, S. (2009). "Formation and Characterization of the Iridium Tetroxide Molecule with Iridium in the Oxidation State +VIII". Angewandte Chemie International Edition 48 (42): 7879–7883. doi:10.1002/anie.200902733. PMID 19593837. Bibcode: 2009ACIE...48.7879G.
25. ↑ Holleman, A. F.; Wiberg, E.; Wiberg, N. (2001). Inorganic Chemistry (1st ed.). Academic Press. ISBN 978-0-12-352651-9. OCLC 47901436.
26. ↑ Esteruelas, Miguel A.; López, Ana M.; Oliván, Montserrat (2016). "Polyhydrides of Platinum Group Metals: Nonclassical Interactions and σ-Bond Activation Reactions". Chemical Reviews 116 (15): 8770–8847. doi:10.1021/acs.chemrev.6b00080. PMID 27268136.
27. ↑ Černý, R.; Joubert, J.-M.; Kohlmann, H.; Yvon, K. (2002). "Mg6Ir2H11, a new metal hydride containing saddle-like IrH5−4 and square-pyramidal IrH4−5 hydrido complexes". Journal of Alloys and Compounds 340 (1–2): 180–188. doi:10.1016/S0925-8388(02)00050-6.Mg6Ir2H11,+a+new+metal+hydride+containing+saddle-like+IrH5−4+and+square-pyramidal+IrH4−5+hydrido+complexes&rft.jtitle=Journal+of+Alloys+and+Compounds&rft.aulast=Černý&rft.aufirst=R.&rft.au=Černý, R.&rft.au=Joubert,+J.-M.&rft.au=Kohlmann,+H.&rft.au=Yvon,+K.&rft.date=2002&rft.volume=340&rft.issue=1–2&rft.pages=180–188&rft_id=info:doi/10.1016/S0925-8388(02)00050-6&rfr_id=info:sid/en.wikibooks.org:Chemistry:Iridium">
28. ↑ Gulliver, D. J.; Levason, W. (1982). "The chemistry of ruthenium, osmium, rhodium, iridium, palladium and platinum in the higher oxidation states". Coordination Chemistry Reviews 46: 1–127. doi:10.1016/0010-8545(82)85001-7.
29. ↑ 29.0 29.1 29.2 29.3 29.4 Renner, H.; Schlamp, G.; Kleinwächter, I.; Drost, E.; Lüschow, H. M.; Tews, P.; Panster, P.; Diehl, M. et al. (2002). "Platinum group metals and compounds". Ullmann's Encyclopedia of Industrial Chemistry. Wiley. doi:10.1002/14356007.a21_075. ISBN 978-3527306732.
30. ↑ Schmidtke, Hans-Herbert (1970). "Pentaammineiridium(III) Complexes". Inorganic Syntheses. 12. pp. 243–247. doi:10.1002/9780470132432.ch42. ISBN 978-0-470-13171-8.
31. ↑ Crabtree, R. H. (1979). "Iridium compounds in catalysis". Accounts of Chemical Research 12 (9): 331–337. doi:10.1021/ar50141a005.
32. ↑ Crabtree, R. H. (2005). The Organometallic Chemistry of the Transition Metals. Wiley. ISBN 978-0471662563. OCLC 224478241. http://chimicibicocca.altervista.org/data/chimica_lucidi.pdf.
33. ↑ Janowicz, A. H.; Bergman, R. G. (1982). "Carbon-hydrogen activation in completely saturated hydrocarbons: direct observation of M + R–H → M(R)(H)". Journal of the American Chemical Society 104 (1): 352–354. doi:10.1021/ja00365a091.
34. ↑ Hoyano, J. K.; Graham, W. A. G. (1982). "Oxidative addition of the carbon-hydrogen bonds of neopentane and cyclohexane to a photochemically generated iridium(I) complex". Journal of the American Chemical Society 104 (13): 3723–3725. doi:10.1021/ja00377a032. Bibcode: 1982JAChS.104.3723H.
35. ↑ Hartwig, John F. (2011). "Regioselectivity of the Borylation of Alkanes and Arenes". Chemical Society Reviews 40 (4): 1992–2002. doi:10.1039/c0cs00156b. PMID 21336364.
36. ↑ 36.0 36.1 36.2 Weeks, Mary Elvira (1932). "The discovery of the elements. VIII. The platinum metals". Journal of Chemical Education (American Chemical Society (ACS)) 9 (6): 1017–1034. doi:10.1021/ed009p1017. ISSN 0021-9584. Bibcode: 1932JChEd...9.1017W. Weeks, M. E. (1968). Discovery of the Elements (7th ed.). Journal of Chemical Education. pp. 385–407. ISBN 978-0-8486-8579-9. OCLC 23991202. https://archive.org/details/discoveryofeleme07edunse.
37. ↑ Donald McDonald, Leslie B. Hunt (1982). A History of Platinum and its Allied Metals. Johnson Matthey Plc. pp. 7–8. ISBN 978-0-905118-83-3.
38. ↑ Dixon, Joshua; Brownrigg, William (1801). The literary life of William Brownrigg. To which are added an account of the coal mines near Whitehaven: And Observations on the means of preventing epidemic fevers. p. 52. https://books.google.com/books?id=525bAAAAQAAJ&pg=PP7.
39. ↑ Watson, Wm; Brownrigg, William (1749). "Several Papers concerning a New Semi-Metal, Called Platina; Communicated to the Royal Society by Mr. Wm. Watson F. R. S". Philosophical Transactions 46 (491–496): 584–596. doi:10.1098/rstl.1749.0110. Bibcode: 1749RSPT...46..584W.
40. ↑ Marggraf, Andreas Sigismund (1760). Versuche mit dem neuen mineralischen Körper Platina del pinto genannt. https://books.google.com/books?id=GWNQAAAAcAAJ.
41. ↑ Thomson, T. (1831). A System of Chemistry of Inorganic Bodies. 1. Baldwin & Cradock, London; and William Blackwood, Edinburgh. p. 693. https://archive.org/details/asystemchemistr07thomgoog.
42. ↑ 42.0 42.1 Griffith, W. P. (2004). "Bicentenary of Four Platinum Group Metals. Part II: Osmium and iridium – events surrounding their discoveries". Platinum Metals Review 48 (4): 182–189. doi:10.1595/147106704x4844. http://www.technology.matthey.com/article/48/4/182-189/.
43. ↑ Weeks, M. E. (1968). Discovery of the Elements (7th ed.). Journal of Chemical Education. pp. 414–418. ISBN 978-0-8486-8579-9. OCLC 23991202. https://archive.org/details/discoveryofeleme0000week.
44. ↑ Tennant, S. (1804). "On Two Metals, Found in the Black Powder Remaining after the Solution of Platina". Philosophical Transactions of the Royal Society of London 94: 411–418. doi:10.1098/rstl.1804.0018. https://zenodo.org/record/1432312.
45. ↑ Trigg, G. L. (1995). "Recoilless Emission and Absorption of Radiation". Landmark Experiments in Twentieth Century Physics. Courier Dover Publications. pp. 179–190. ISBN 978-0-486-28526-9. OCLC 31409781. https://books.google.com/books?id=YOQ9fi5yQ4sC.
46. ↑ Mössbauer, R. L. (1958). "Gammastrahlung in Ir191" (in de). Zeitschrift für Physik A 151 (2): 124–143. doi:10.1007/BF01344210. Bibcode: 1958ZPhy..151..124M.
47. ↑ Waller, I. (1964). "The Nobel Prize in Physics 1961: presentation speech". Nobel Lectures, Physics 1942–1962. Elsevier. http://nobelprize.org/nobel_prizes/physics/laureates/1961/press.html.
48. ↑ "History/Origin of Chemicals". NASA. http://herschel.jpl.nasa.gov/chemicalOrigins.shtml.
49. ↑ Chen, Hsin-Yu; Vitale, Salvatore; Foucart, Francois (2021-10-01). "The Relative Contribution to Heavy Metals Production from Binary Neutron Star Mergers and Neutron Star–Black Hole Mergers". The Astrophysical Journal Letters (American Astronomical Society) 920 (1): L3. doi:10.3847/2041-8213/ac26c6. ISSN 2041-8205. Bibcode: 2021ApJ...920L...3C.
50. ↑ Arlandini, Claudio; Kappeler, Franz; Wisshak, Klaus; Gallino, Roberto; Lugaro, Maria; Busso, Maurizio; Straniero, Oscar (1999-11-10). "Neutron Capture in Low-Mass Asymptotic Giant Branch Stars: Cross Sections and Abundance Signatures" (in en). The Astrophysical Journal 525 (2): 886–900. doi:10.1086/307938. ISSN 0004-637X. Bibcode: 1999ApJ...525..886A. https://iopscience.iop.org/article/10.1086/307938.
51. ↑ Scott, E. R. D.; Wasson, J. T.; Buchwald, V. F. (1973). "The chemical classification of iron meteorites—VII. A reinvestigation of irons with Ge concentrations between 25 and 80 ppm". Geochimica et Cosmochimica Acta 37 (8): 1957–1983. doi:10.1016/0016-7037(73)90151-8. Bibcode: 1973GeCoA..37.1957S.
52. ↑ "Abundance of Elements in the Earth's Crust and in the Sea". CRC Handbook of Chemistry and Physics (97th ed.). CRC Press. 2017. pp. 14–17. ISBN 978-1-4987-5429-3. https://archive.org/details/CRCHandbookOfChemistryAndPhysics97thEdition2016/page/n2401.
53. ↑ 53.0 53.1 "Iridium". Human Health Fact Sheet. Argonne National Laboratory. 2005. http://www.ead.anl.gov/pub/doc/Iridium.pdf.
54. ↑ Xiao, Z.; Laplante, A. R. (2004). "Characterizing and recovering the platinum group minerals—a review". Minerals Engineering 17 (9–10): 961–979. doi:10.1016/j.mineng.2004.04.001. Bibcode: 2004MiEng..17..961X.
55. ↑ "Cuproiridsite CuIr2S4". http://www.handbookofmineralogy.org/pdfs/cuproiridsite.pdf.
56. ↑ Vitaly A. Stepanov; Valentina E. Kungurova; Vitaly I. Gvozdev (2010). "Irasite Discovery in Copper-Nickel Ores of Shanuch Deposit (KAMCHATKA)". New Data on Minerals 45: 23. https://www.fmm.ru/images/8/89/NDM_2010_45_Stepanov_eng.pdf. Retrieved 3 March 2022.
57. ↑ Garuti, Giorgio; Gazzotti, Moreno; Torres-Ruiz, Jose (1995). "Iridium, Rhodium, and Platinum Sulfides in Chromitites from the Ultramafic Massifs of Finero, Italy, and Ojen, Spain". The Canadian Mineralogist 33: 509–520. https://rruff.info/uploads/CM33_509.pdf. Retrieved 2 November 2022.
58. ↑ 58.0 58.1 58.2 58.3 Seymour, R. J.; O'Farrelly, J. I. (2012). "Platinum-Group Metals". Kirk Othmer Encyclopedia of Chemical Technology. Wiley. doi:10.1002/0471238961.1612012019052513.a01.pub3. ISBN 978-0471238966.
59. ↑ 59.0 59.1 Goldberg, Hodge; Kay, V; Stallard, M; Koide, M (1986). "Some comparative marine chemistries of platinum and iridium". Applied Geochemistry 1 (2): 227–232. doi:10.1016/0883-2927(86)90006-5. Bibcode: 1986ApGC....1..227G.
60. ↑ 60.0 60.1 60.2 Wells, Boothe (1988). "Iridium in marine organisms". Geochimica et Cosmochimica Acta 52 (6): 1737–1739. doi:10.1016/0016-7037(88)90242-6. Bibcode: 1988GeCoA..52.1737W.
61. ↑ 61.0 61.1 61.2 Sawlowicz, Z (1993). "Iridium and other platinum-group elements as geochemical markers in sedimentary environments". Palaeogeography, Palaeoclimatology, Palaeoecology 104 (4): 253–270. doi:10.1016/0031-0182(93)90136-7. Bibcode: 1993PPP...104..253S.
62. ↑ Crocket, Macdougall; Harriss, R (1973). "Gold, palladium and iridium in marine sediments". Geochimica et Cosmochimica Acta 37 (12): 2547–2556. doi:10.1016/0016-7037(73)90264-0. Bibcode: 1973GeCoA..37.2547C.
63. ↑ Peucker-Ehrenbrink, B (2001). "Iridium and Osmium as Tracers of Extraterrestrial Matter in Marine Sediments". Accretion of Extraterrestrial Matter Throughout Earth's History. pp. 163–178. doi:10.1007/978-1-4419-8694-8_10. ISBN 978-1-4613-4668-5.
64. ↑ Barker, J; Edward, A (1968). "Accretion rate of cosmic matter from iridium and osmium contents of deep-sea sediments". Geochimica et Cosmochimica Acta 32 (6): 627–645. doi:10.1016/0016-7037(68)90053-7. Bibcode: 1968GeCoA..32..627B.
65. ↑ Colodner, D; Edmond, J (1992). "Post-depositional mobility of platinum, iridium and rhenium in marine sediments". Nature 358 (6385): 402–404. doi:10.1038/358402a0. Bibcode: 1992Natur.358..402C.
66. ↑ 66.0 66.1 Alvarez, L. W.; Alvarez, W.; Asaro, F.; Michel, H. V. (1980). "Extraterrestrial cause for the Cretaceous–Tertiary extinction". Science 208 (4448): 1095–1108. doi:10.1126/science.208.4448.1095. PMID 17783054. Bibcode: 1980Sci...208.1095A. http://chaos.swarthmore.edu/courses/soc26/bak-sneppan/13_alverez.pdf.
67. ↑ Hildebrand, A. R.; Penfield, Glen T.; Kring, David A.; Pilkington, Mark; Zanoguera, Antonio Camargo; Jacobsen, Stein B.; Boynton, William V. (1991). "Chicxulub Crater; a possible Cretaceous/Tertiary boundary impact crater on the Yucatan Peninsula, Mexico". Geology 19 (9): 867–871. doi:10.1130/0091-7613(1991)019<0867:CCAPCT>2.3.CO;2. Bibcode: 1991Geo....19..867H.
68. ↑ Frankel, C. (1999). The End of the Dinosaurs: Chicxulub Crater and Mass Extinctions. Cambridge University Press. ISBN 978-0-521-47447-4. OCLC 40298401. https://archive.org/details/endofdinosaursch00fran.
69. ↑ Ryder, G.; Fastovsky, D. E.; Gartner, S. (1996). The Cretaceous-Tertiary Event and Other Catastrophes in Earth History. Geological Society of America. p. 47. ISBN 978-0-8137-2307-5.
70. ↑ Toutain, J.-P.; Meyer, G. (1989). "Iridium-Bearing Sublimates at a Hot-Spot Volcano (Piton De La Fournaise, Indian Ocean)". Geophysical Research Letters 16 (12): 1391–1394. doi:10.1029/GL016i012p01391. Bibcode: 1989GeoRL..16.1391T.
71. ↑ 71.0 71.1 71.2 Platinum-Group Metals. U.S. Geological Survey Mineral Commodity Summaries
72. ↑ Singerling, Sheryl A.; Schulte, Ruth F. (August 2021). "Platinum-Group Metals". 2018 Minerals Yearbook. USGS. p. 57.11. https://d9-wret.s3.us-west-2.amazonaws.com/assets/palladium/production/atoms/files/myb1-2018-plati.pdf.
73. ↑ Hagelüken, C. (2006). "Markets for the catalysts metals platinum, palladium, and rhodium". Metall 60 (1–2): 31–42. http://www.preciousmetals.umicore.com/publications/articles_by_umicore/general/show_Metal_PGMmarkets_200602.pdf.
74. ↑ "Platinum 2013 Interim Review". Johnson Matthey. http://www.platinum.matthey.com/media/1631250/other_pgm.pdf.
75. ↑ 75.0 75.1 Ryan, Marge (2022-11-16). "Recycling and thrifting: the answer to the iridium question in electrolyser growth". https://matthey.com/en/iridium-supply-hydrogen-electrolysers.
76. ↑ Gilchrist, Raleigh (1943). "The Platinum Metals". Chemical Reviews 32 (3): 277–372. doi:10.1021/cr60103a002.
77. ↑ Ohriner, E. K. (2008). "Processing of Iridium and Iridium Alloys". Platinum Metals Review 52 (3): 186–197. doi:10.1595/147106708X333827.
78. ↑ Hunt, L. B.; Lever, F. M. (1969). "Platinum Metals: A Survey of Productive Resources to industrial Uses". Platinum Metals Review 13 (4): 126–138. doi:10.1595/003214069X134126138. http://www.platinummetalsreview.com/pdf/pmr-v13-i4-126-138.pdf. Retrieved 2008-10-01.
79. ↑ "Mineral Yearbook 2020 tables-only release". https://www.usgs.gov/centers/national-minerals-information-center/platinum-group-metals-statistics-and-information.
80. ↑ 80.0 80.1 Handley, J. R. (1986). "Increasing Applications for Iridium". Platinum Metals Review 30 (1): 12–13. doi:10.1595/003214086X3011213. https://technology.matthey.com/article/30/1/12-13/.
81. ↑ Crookes, W. (1908). "On the Use of Iridium Crucibles in Chemical Operations". Proceedings of the Royal Society of London. Series A, Containing Papers of a Mathematical and Physical Character 80 (541): 535–536. doi:10.1098/rspa.1908.0046. Bibcode: 1908RSPSA..80..535C.
82. ↑ Egorova, R. V.; Korotkov, B. V.; Yaroshchuk, E. G.; Mirkus, K. A.; Dorofeev N. A.; Serkov, A. T. (1979). "Spinnerets for viscose rayon cord yarn". Fibre Chemistry 10 (4): 377–378. doi:10.1007/BF00543390.
83. ↑ Graff, Muriel; Kempf, Bernd; Breme, Jürgen (2005-12-23). "Iridium Alloy for Spark Plug Electrodes". Materials for Transportation Technology. Weinheim, FRG: Wiley-VCH Verlag GmbH & Co. KGaA. pp. 1–8. doi:10.1002/3527606025.ch1. ISBN 9783527301249.
84. ↑ Cheung, H.; Tanke, R. S.; Torrence, G. P. (2000). "Acetic acid". Ullmann's Encyclopedia of Industrial Chemistry. Wiley. doi:10.1002/14356007.a01_045. ISBN 978-3527306732.
85. ↑ Jones, Jane H. (2000). "The cativa™ process for the manufacture of acetic acid.". Platinum Metals Review 44 (3): 94–105. doi:10.1595/003214000X44394105. https://technology.matthey.com/article/44/3/94-105/.
86. ↑ Roseblade, S. J.; Pfaltz, A. (2007). "Iridium-catalyzed asymmetric hydrogenation of olefins". Accounts of Chemical Research 40 (12): 1402–1411. doi:10.1021/ar700113g. PMID 17672517.
87. ↑ Ikariya, Takao; Blacker, A. John (2007). "Asymmetric Transfer Hydrogenation of Ketones with Bifunctional Transition Metal-Based Molecular Catalysts†". Accounts of Chemical Research 40 (12): 1300–1308. doi:10.1021/ar700134q. PMID 17960897.
88. ↑ Matthias Beller, Hans-Ulrich Blaser, ed (2012). Organometallics as Catalysts in the Fine Chemical Industry. Topics in Organometallic Chemistry. 42. Berlin, Heidelberg: Springer. ISBN 978-3-642-32832-9.
89. ↑ Halmshaw, R. (1954). "The use and scope of Iridium 192 for the radiography of steel". British Journal of Applied Physics 5 (7): 238–243. doi:10.1088/0508-3443/5/7/302. Bibcode: 1954BJAP....5..238H.
90. ↑ Hellier, Chuck (2001). Handbook of Nondestructive Evlaluation. The McGraw-Hill Companies. ISBN 978-0-07-028121-9.
91. ↑ Jean Pouliot; Luc Beaulieu (2010). "13 – Modern Principles of Brachytherapy Physics: From 2-D to 3-D to Dynamic Planning and Delivery". Leibel and Phillips Textbook of Radiation Oncology (3rd ed.). W.B. Saunders. pp. 224–244. doi:10.1016/B978-1-4160-5897-7.00013-5. ISBN 9781416058977. https://www.sciencedirect.com/topics/medicine-and-dentistry/iridium-192.
92. ↑ Ulbricht, Christoph; Beyer, Beatrice; Friebe, Christian; Winter, Andreas; Schubert, Ulrich S. (2009). "Recent Developments in the Application of Phosphorescent Iridium(III) Complex Systems". Advanced Materials 21 (44): 4418–4441. doi:10.1002/adma.200803537. Bibcode: 2009AdM....21.4418U.
93. ↑ Penzes, W. B. (2001). "Time Line for the Definition of the Meter". National Institute for Standards and Technology. https://www.nist.gov/document/museum-timelinepdf.
94. ↑ General section citations: Recalibration of the U.S. National Prototype Kilogram, R. S. Davis, Journal of Research of the National Bureau of Standards, 90, No. 4, July–August 1985 (5.5 MB PDF ); and The Kilogram and Measurements of Mass and Force, Z. J. Jabbour et al., J. Res. Natl. Inst. Stand. Technol. 106, 2001, 25–46 (3.5 MB PDF)
95. ↑ Mottishaw, J. (1999). "Notes from the Nib Works—Where's the Iridium?". The PENnant XIII (2). https://www.nibs.com/blog/nibster-writes/wheres-iridium. Retrieved 2022-09-24.
96. ↑ Crookes, W., ed (1867). "The Paris Exhibition". The Chemical News and Journal of Physical Science XV: 182. https://en.wikisource.org/w/index.php?title=File:The_chemical_news._Volume_15,_January_-_June_1867._(IA_s713id13683370).pdf&page=188.
97. ↑ Pepper, J. H. (1861). The Playbook of Metals: Including Personal Narratives of Visits to Coal, Lead, Copper, and Tin Mines, with a Large Number of Interesting Experiments Relating to Alchemy and the Chemistry of the Fifty Metallic Elements. Routledge, Warne, and Routledge. p. 455. https://archive.org/details/playbookmetalsi00peppgoog.
98. ↑ "Iridium (Ir) – Chemical properties, Health and Environmental effects". https://www.lenntech.com/periodic/elements/ir.htm#:~:text=not been estimated.-,Health effects of iridium,irritation of the digestive tract..
99. ↑ "Radioisotope Brief: Iridium-192 (Ir-192)". Radiation Emergencies. Centers for Disease Control and Prevention. 2004-08-18. http://emergency.cdc.gov/radiation/isotopes/pdf/iridium.pdf.

## External links

| Wikimedia Commons has media related to Iridium.

|

* Iridium at The Periodic Table of Videos (University of Nottingham)
* Iridium in Encyclopædia Britannica

* v
* t
* e

Periodic table

|  | 1 | 2 |  | 3 | 4 | 5 | 6 | 7 | 8 | 9 | 10 | 11 | 12 | 13 | 14 | 15 | 16 | 17 | 18

|
|
|
|
|
|
|
|
|
|
|
|
|
|
|
|
|
|
|

1 | H |  | He
2 | Li | Be |  | B | C | N | O | F | Ne
3 | Na | Mg |  | Al | Si | P | S | Cl | Ar
4 | K | Ca |  | Sc | Ti | V | Cr | Mn | Fe | Co | Ni | Cu | Zn | Ga | Ge | As | Se | Br | Kr
5 | Rb | Sr |  | Y | Zr | Nb | Mo | Tc | Ru | Rh | Pd | Ag | Cd | In | Sn | Sb | Te | I | Xe
6 | Cs | Ba | La | Ce | Pr | Nd | Pm | Sm | Eu | Gd | Tb | Dy | Ho | Er | Tm | Yb | Lu | Hf | Ta | W | Re | Os | Ir | Pt | Au | Hg | Tl | Pb | Bi | Po | At | Rn
7 | Fr | Ra | Ac | Th | Pa | U | Np | Pu | Am | Cm | Bk | Cf | Es | Fm | Md | No | Lr | Rf | Db | Sg | Bh | Hs | Mt | Ds | Rg | Cn | Nh | Fl | Mc | Lv | Ts | Og

| Alkali metal | Alkaline earth metal | Lan­thanide | Actinide | Transition metal | Post-​transition metal | Metalloid | Reactive nonmetal | Noble gas

|
|
|
|
|
|
|
|

* v
* t
* e

Iridium compounds

Iridium(0)|

| Organoiridium(0)|

* Ir4(CO)12

|

Iridium(I)|

| Organoiridium(I)|

* IrC8H12C5H5NP(C6H11)3PF6
* IrClCO(P(C6H5)3)2
* KIrI2(CO)2

|

Iridium(III)|

* IrCl3

| Organoiridium(III)|

* (IrClC5(CH3)5)2Cl2

|

Iridium(IV)|

* IrF4
* IrO2
* (NH4)2[IrCl6]

Iridium(V)|

* IrF5

Iridium(VI)|

* IrF6

Iridium(VII)|

* IrF7

Iridium(VIII)|

* IrO4

0.00

(0 votes)

Original source: https://en.wikipedia.org/wiki/Iridium. Read more

|

Retrieved from "https://handwiki.org/wiki/index.php?title=Chemistry:Iridium&oldid=4031851"
*[v]: View this template
*[t]: Discuss this template
*[e]: Edit this template